Download presentation

1
**Homogeneous Semiconductors**

Dopants Use Density of States and Distribution Function to: Find the Number of Holes and Electrons.

2
**Energy Levels in Hydrogen Atom**

3
**Energy Levels for Electrons in a Doped Semiconductor**

4
**Assumptions for Calculation**

8
Density of States (Appendix D) Energy Distribution Functions (Section 2.9) Carrier Concentrations (Sections )

9
**GOAL: The density of electrons (no) can be found precisely if we know**

1. the number of allowed energy states in a small energy range, dE: S(E)dE “the density of states” 2. the probability that a given energy state will be occupied by an electron: f(E) “the distribution function” no = bandS(E)f(E)dE

10
**For quasi-free electrons in the conduction band: 1**

For quasi-free electrons in the conduction band: 1. We must use the effective mass (averaged over all directions) 2. the potential energy Ep is the edge of the conduction band (EC) For holes in the valence band: 1. We still use the effective mass (averaged over all directions) 2. the potential energy Ep is the edge of the valence band (EV)

11
**Energy Band Diagram E(x) Eelectron S(E) Ehole x**

conduction band valence band EC EV x E(x) Eelectron S(E) Ehole note: increasing electron energy is ‘up’, but increasing hole energy is ‘down’.

12
Reminder of our GOAL: The density of electrons (no) can be found precisely if we know 1. the number of allowed energy states in a small energy range, dE: S(E)dE “the density of states” 2. the probability that a given energy state will be occupied by an electron: f(E) “the distribution function” no = bandS(E)f(E)dE

13
**Fermi-Dirac Distribution**

The probability that an electron occupies an energy level, E, is f(E) = 1/{1+exp[(E-EF)/kT]} where T is the temperature (Kelvin) k is the Boltzmann constant (k=8.62x10-5 eV/K) EF is the Fermi Energy (in eV) (Can derive this – statistical mechanics.)

14
**f(E) = 1/{1+exp[(E-EF)/kT]}**

EF E T=0 oK T1>0 T2>T1 0.5 All energy levels are filled with e-’s below the Fermi Energy at 0 oK

15
**Fermi-Dirac Distribution for holes**

Remember, a hole is an energy state that is NOT occupied by an electron. Therefore, the probability that a state is occupied by a hole is the probability that a state is NOT occupied by an electron: fp(E) = 1 – f(E) = 1 - 1/{1+exp[(E-EF)/kT]} ={1+exp[(E-EF)/kT]}/{1+exp[(E-EF)/kT]} /{1+exp[(E-EF)/kT]} = {exp[(E-EF)/kT]}/{1+exp[(E-EF)/kT]} =1/{exp[(EF - E)/kT] + 1} for the last line, multiply by 1 = exp(-(E-Ef)/kT)/exp(-(E-Ef)/kT)

16
**The Boltzmann Approximation If (E-EF)>kT such that exp[(E-EF)/kT] >> 1 then,**

f(E) = {1+exp[(E-EF)/kT]}-1 {exp[(E-EF)/kT]}-1 exp[-(E-EF)/kT] …the Boltzmann approx. similarly, fp(E) is small when exp[(EF - E)/kT]>>1: fp(E) = {1+exp[(EF - E)/kT]}-1 {exp[(EF - E)/kT]}-1 exp[-(EF - E)/kT] If the Boltz. approx. is valid, we say the semiconductor is non-degenerate.

17
**Putting the pieces together: for electrons, n(E)**

f(E) 1 EF E T=0 oK T1>0 T2>T1 0.5 EV EC S(E) E n(E)=S(E)f(E)

18
**Putting the pieces together:**

for holes, p(E) fp(E) T=0 oK 1 T1>0 T2>T1 0.5 S(E) E EV EF EC p(E)=S(E)f(E) hole energy

19
**Finding no and po the effective density of states**

in the conduction band

20
**Energy Band Diagram intrinisic semiconductor: no=po=ni**

E(x) conduction band EC n(E) EF=Ei p(E) EV valence band x where Ei is the intrinsic Fermi level

21
**Energy Band Diagram n-type semiconductor: no>po**

E(x) conduction band EC EF n(E) p(E) EV valence band x

22
**Energy Band Diagram p-type semiconductor: po>no**

E(x) conduction band EC n(E) p(E) EF EV valence band x

23
**A very useful relationship**

…which is independent of the Fermi Energy Recall that ni = no= po for an intrinsic semiconductor, so nopo = ni2 for all non-degenerate semiconductors. (that is as long as EF is not within a few kT of the band edge)

24
**The intrinsic carrier density**

is sensitive to the energy bandgap, temperature, and m*

25
**The intrinsic Fermi Energy (Ei)**

For an intrinsic semiconductor, no=po and EF=Ei which gives Ei = (EC + EV)/2 + (kT/2)ln(NV/NC) so the intrinsic Fermi level is approximately in the middle of the bandgap.

37
**no = 0.5(ND-NA) 0.5[(ND-NA)2 + 4ni2]1/2**

Higher Temperatures Consider a semiconductor doped with NA ionized acceptors (-q) and ND ionized donors (+q), do not assume that ni is small – high temperature expression. positive charges = negative charges po + ND = no + NA using ni2 = nopo ni2/no + ND = no+ NA ni2 + no(ND-NA) - no2 = 0 no = 0.5(ND-NA) 0.5[(ND-NA)2 + 4ni2]1/2 we use the ‘+’ solution since no should be increased by ni no = ND - NA in the limit that ni<<ND-NA

38
**Temperature variation of some important “constants.”**

Simpler Expression

44
**Degenerate Semiconductors**

1. The doping concentration is so high that EF moves within a few kT of the band edge (EC or EV). Boltzman approximation not valid. 2. High donor concentrations cause the allowed donor wavefunctions to overlap, creating a band at Edn. First only the high states overlap, but eventually even the lowest state overlaps. This effectively decreases the bandgap by DEg = Eg0 – Eg(ND). EC EV + ED1 Eg0 Eg(ND) for ND > 1018 cm-3 in Si impurity band

45
**Degenerate Semiconductors**

As the doping conc. increases more, EF rises above EC EV EC (intrinsic) available impurity band states EF DEg EC (degenerate) ~ ED filled impurity band states apparent band gap narrowing: DEg* (is optically measured) - Eg* is the apparent band gap: an electron must gain energy Eg* = EF-EV

46
**Electron Concentration in degenerately doped n-type semiconductors**

The donors are fully ionized: no = ND The holes still follow the Boltz. approx. since EF-EV>>>kT po = NV exp[-(EF-EV)/kT] = NV exp[-(Eg*)/kT] = NV exp[-(Ego- DEg*)/kT] = NV exp[-Ego/kT]exp[DEg*)/kT] nopo = NDNVexp[-Ego/kT] exp[DEg*)/kT] = (ND/NC) NCNVexp[-Ego/kT] exp[DEg*)/kT] = (ND/NC)ni2 exp[DEg*)/kT]

47
**Summary non-degenerate: nopo= ni2 degenerate n-type:**

nopo= ni2 (ND/NC) exp[DEg*)/kT] degenerate p-type: nopo= ni2 (NA/NV) exp[DEg*)/kT]

Similar presentations

OK

Lecture #3 OUTLINE Band gap energy Density of states Doping Read: Chapter 2 (Section 2.3)

Lecture #3 OUTLINE Band gap energy Density of states Doping Read: Chapter 2 (Section 2.3)

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on general knowledge quiz Ppt on land and sea breeze Ppt on fdi in hindi Ppt on sports day logo Ppt on water bodies on earth Ppt on ideal gas law practice Ppt on low level language in computer Ppt on green building design Ppt on gender inequality in india Nano emissive display ppt online